of 47

• date post

08-Mar-2015
• Category

## Documents

• view

73

3

Embed Size (px)

### Transcript of Xrd Presentation Basics

X-ray Diffraction (XRD) 1.0 What is X-ray Diffraction 2.0 Basics of Crystallography 3.0 Production of X-rays 4.0 Applications of XRD 5.0 Instrumental Sources of Error 6.0 Conclusions

Braggs Law

n =2dsinEnglish physicists Sir W.H. Bragg and his son Sir W.L. Bragg developed a relationship in 1913 to explain why the cleavage faces of crystals appear to reflect X-ray beams at certain angles of incidence (theta, ). The variable d is the distance between atomic layers in a crystal, and the variable lambda is the wavelength of the incident X-ray beam; n is an integer. This observation is an example of X-ray wave interference (Roentgenstrahlinterferenzen), commonly known as X-ray diffraction (XRD), and was direct evidence for the periodic atomic structure of crystals postulated for several centuries.

Braggs Law

n =2dsinThe Braggs were awarded the Nobel Prize in physics in 1915 for their work in determining crystal structures beginning with NaCl, ZnS and diamond.

Although Bragg's law was used to explain the interference pattern of X-rays scattered by crystals, diffraction has been developed to study the structure of all states of matter with any beam, e.g., ions, electrons, neutrons, and protons, with a wavelength similar to the distance between the atomic or molecular structures of interest.

Deriving Braggs Law: n = 2dsinX-ray 1

Constructive interference occurs only when n = AB + BC AB=BC n = 2AB Sin=AB/d AB=dsin n =2dsin

X-ray 2

AB+BC = multiples of n

= 2dhklsinhkl

Constructive and Destructive Interference of Waves

Constructive Interference In Phase

Destructive Interference Out of Phase

1.0 What is X-ray Diffraction ? I

www.micro.magnet.fsu.edu/primer/java/interference/index.html

Why XRD? Measure the average spacings between layers or rows of atoms Determine the orientation of a single crystal or grain Find the crystal structure of an unknown material Measure the size, shape and internal stress of small crystalline regions

X-ray Diffraction (XRD)The atomic planes of a crystal cause an incident beam of X-rays to interfere with one another as they leave the crystal. The phenomenon is called X-ray diffraction.

incident beam

Effect of sample thickness on the absorption of X-raysdiffracted beam film

crystal

http://www.matter.org.uk/diffraction/x-ray/default.htm

Detection of Diffracted X-raysby Photographic filmsample film

X-rayPoint where incident beam enters 2 = 180

Film2 = 0

Debye - Scherrer CameraA sample of some hundreds of crystals (i.e. a powdered sample) show that the diffracted beams form continuous cones. A circle of film is used to record the diffraction pattern as shown. Each cone intersects the film giving diffraction lines. The lines are seen as arcs on the film.

Braggs Law and Diffraction:How waves reveal the atomic structure of crystals

n = 2dsinX-ray1 X-ray2

n-integer

Diffraction occurs only when Braggs Law is satisfied Condition for constructive interference (X-rays 1 & 2) from planes with spacing d

=3 d=3

l=30o

Atomic plane

2-diffraction angle

http://www.eserc.stonybrook.edu/ProjectJava/Bragg/

Planes in Crystals-2 dimension = 2dhklsinhkl

Different planes have different spacings

To satisfy Braggs Law, must change as d changes e.g., decreases as d increases.

2.0 Basics of Crystallographysmallest building block

c

d3 a b

Unit cell ()Beryl crystals

CsCl

d1 Lattice d2

(cm)

A crystal consists of a periodic arrangement of the unit cell into a lattice. The unit cell can contain a single atom or atoms in a fixed arrangement. Crystals consist of planes of atoms that are spaced a distance d apart, but can be resolved into many atomic planes, each with a different dspacing. a,b and c (length) and , and angles between a,b and c are lattice constants or parameters which can be determined by XRD.

Seven Crystal Systems - Review

Miller Indices: hkl - ReviewMiller indices-the reciprocals of the fractional intercepts which the plane makes with crystallographic axes

(010)

Axial length Intercept lengths Fractional intercepts Miller indices

a b c 4 8 3 1 4 3 1 4 2 1 h k l

a b c 4 8 3 8 0 1 0 0 1 0 h k l4/ =0

Several Atomic Planes and Their d-spacings in a Simple Cubic - Reviewa b c 1 0 0 1 0 0 d100 a b c 1 1 0 1 1 0

(100)a b c 1 1 1 1 1 1

Cubica=b=c=a0

(110)a b c 0 1 0 1 2

d012

(111)

(012)

Black numbers-fractional intercepts, Blue numbers-Miller indices

Planes and Spacings - Review

Indexing of Planes and Directions Reviewc (111) c

b a a

b [110]

a direction: [uvw] : a set of equivalent directions

a plane: (hkl) {hkl}: a set of equivalent planes

3.0 Production of X-raysCross section of sealed-off filament X-ray tubecopper X-rays vacuumtungsten filament glass

cooling water

electrons

to transformer

target Vacuumberyllium window metal focusing cap

X-rays

X-rays are produced whenever high-speed electrons collide with a metal target. A source of electrons hot W filament, a high accelerating voltage between the cathode (W) and the anode and a metal target, Cu, Al, Mo, Mg. The anode is a water-cooled block of Cu containing desired target metal.

Characteristic X-ray LinesK K and K2 will cause extra peaks in XRD pattern, and shape changes, but can be eliminated by adding filters. ----- is the mass absorption coefficient of Zr.

Intensity

K1